AISI 1045 steel Manufacturer and Exporter,you can get round,square,flat,block,and shaft etc.
- AISI 1045 is defined as medium carbon steel, AISI 1045 steel has 0.43%-0.5% Carbon.
- AISI 1045offers good weldability, good machinability, high strength and impact properties.
- AISI 1045 islow in hardenability, because of lack of suitable alloying elements.
- AISI 1045can obtain surface hardnesses 54-60HRC after flame or induction hardening.
- AISI 1045 is generally supplied in the black hot forged or normalized condition,and has a tensile strength of 570 -700 MPa with surfacehardness170-210HB.
|Φ6-Φ100||Cold Drawn||Bright/Black||Best H11|
|Flat/Square/Block||Thickness :120-800||Hot Forged||Black||-0/+8mm|
1.Supply Form & Size & Tolerance
Remark:Tolerance can be customized as per requests
|Melting point °C||1495|
|Modulus of Elasticity, psi||29 x 10^6|
|Coefficient of Thermal Expansion, 68-212˚F, /˚F||6.39 x 10^-6|
|Thermal Conductivity, Btu/ft hr ˚F||30|
|Specific Heat, Btu/lb ˚F||0.116|
|Electrical Resistivity, Microhm-in||6.42|
|Section Size mm||≤ 16||17 – 40||41 – 100|
|Tensile Strength Mpa||700-850||6500-800||630-780|
|Yield Strength Mpa||≥ 500||≥430||≥ 370|
|Elongation in 50mm %||≥ 14||≥ 16||≥ 17|
|Impact Charpy J||≥ 30||≥ 30||≥ 30|
Remark:Water Quench at 820 oC -850 oC or oil quench at 830 °C-860°C and Tempered Between 540 °C – 680 °C
Heat AISI 1045 with two steps,first heat the temperature to 750 oC – 800 oC ,hold for suitable time,then heat the temperature up to 1100 oC – 1200 oC,hold enough time for the steel to be thoroughly heated.Minimum forging temperature 850°C,so don’t forge below it.AISI 1045 steel should be cooled as slowly as possible in still air or in sand after forged.
Normalizing is used to refine the structure of forgings that might have cooled non-uniformly after forged,and considered as a conditioning treatment before final heat treatment.Normalizing temperature for AISI 1045 steel should be carried out between 870℃-920℃. hold suitable time for the steel to be thoroughly heated to complete the ferrite to austenite transformation.Soak for 10 – 15 minutes,then cool in still air.
Annealing is considered as a treatment suitable for machining.AISI 1045 should be carried our at a nominal temperature of 800℃-850℃,hold suitable time for the steel to be thoroughly heated, then furnace cooling.
AISI 1045 may be hardened to increase surface hardness and strength.It is usually heated to temperature 820oC – 860oC,hold suitable time for the steel to be heated uniformly,soak for 10 -15 minutes per 25mm of section, and quench in water or oil.Tempering should be followed immediately after quenched.
Tempering will be carried out to optimize the property after quench.AISI 1045 steel is usually heated to 400oC – 650oC as required, hold until temperature is uniform throughout the section, soak for 1 hour per 25mm of section, and cool in still air.
Compared with AISI 1020,AISI 1045 has low alloy,but can be flamed or induction hardening to obtain high strength,and is widely used in many industries which require more strength,wear resistance,
Typical applications includes Axles,Bolts, Connecting Rods, Hydraulic Clamps ,Rams, Pins , Rolls, Studs, Shafts, Spindles, Sockets, Light gears etc.